# optical properties of cdse nanocrystals jmlvll/lab-reports/cdse/cdse.pdfuc berkeley college of...

Post on 29-May-2018

213 views

Embed Size (px)

TRANSCRIPT

UC Berkeley College of Chemistry

Chemistry 125

Physical Chemistry Laboratory

Optical Properties of CdSeNanocrystals

Author:

Jonathan Melville

Lab Partner:

David Gygi

Graduate Student Instructor:

Marieke Jager

November 21, 2014

1 Observations

Sample Time Removed Color Color under UVSample 1 10.41 sec. Yellow Blue-greenSample 2 20.60 sec. Gold Bright aquamarineSample 3 29.98 sec. Orange GreenSample 4 87.46 sec. Red-orange Red-orangeSample 5 111.90 sec. Red-orange Red-orangeSample 6 118.68 sec. Red Red

Table 1: The colors of nanocrystal solutions under both visible and UV light, in terms ofthe amount of time they were allowed to react before being extracted.

1

Figure 1: The nanocrystal samples, in order.

Figure 2: The nanocrystal samples fluorescing under UV radiation.

2

2 Raw Spectra

2.1 Absorption Spectra

Figure 3: Absorbance spectra overlaid for all six nanocrystal samples.

Figure 4: Absorbance spectra overlaid for all six nanocrystal samples, normalized to havethe same max peak height.

3

2.2 Emission Spectra

Figure 5: Emission spectra overlaid for all six nanocrystal samples.

Figure 6: Emission spectra overlaid for all six nanocrystal samples, normalized to havethe same max peak height. This has drastically increased the noise levels for some of thesamples.

4

3 Collated Emission/Absorption Peak Values

Sample Max Absorbance (nm) Max Emission (nm)Sample 1 487(3) 523(1)Sample 2 504(3) 537(1)Sample 3 515(2) 543(1)Sample 4 528(2) 566(1)Sample 5 534(2) 582(2)Sample 6 537(2) 585(2)

Table 2: Peak absorbance and emission values for all six nanocrystal samples. Uncertain-ties in the last decimal place, in parentheses, were defined by instrumental parameters.

Figure 7: A plot of absorbance vs. emission data for all six nanocrystal samples, with afit by Excels LINEST().

4 Nanoparticle Size Calculation

The following polynomial fit for CdSe nanocrystal size was determined experimentally in

Yu et. al.[1]:

D = 1.6122 1094 2.6575 1063 + 1.6242 1032 0.4277+ 41.57,

5

where D is the diameter of the nanocrystal in nanometers, and is the wavelength of

the nanocrystals first absorbance peak.

The uncertainty propagation equation for this equation is

D =

(4(

)(1.6122 109))2 + (3(

)(2.6575 106))2 + (2(

)(1.6242 103))2 + ((

)(0.4277))2

Using this equation, the following nanocrystal radii and uncertainties can be deter-

mined:

Sample Nanocrystal Radius (nm)Sample 1 1.12(1)Sample 2 1.19(1)Sample 3 1.25(1)Sample 4 1.33(1)Sample 5 1.38(2)Sample 6 1.40(2)

Table 3: Nanocrystal radii, calculated from their absorbance peaks and anexperimentally-determined polynomial.

Figure 8: A plot of nanocrystal radius against the time each sample was reacted for(Table 1 on page 1).

6

5 Nanocrystal Excitation Energy Calculation

The lowest-energy excitation for the nanocrystals synthesized can be calculated using the

following modified particle-in-a-box equation:

Eex =h2

8R2

(1

me+

1

mh

) 1.8e

2

4CdSe0R+ Epol,

where, in addition to an array of fundamental constants, Eex is the excitation energy

of the nanocrystal, R is the radius of the nanocrystal, me is the mass of an electron in a

CdSe exciton (approximately 0.13 times the free-electron mass), mh is the mass of a hole

in a CdSe exciton (approximately 0.45 times the free-electron mass), CdSe is the bulk

dielectric constant for CdSe (approximately 10.6), and Epol is a complex function that

accounts for the polarization of a nanocrystal by an internal point charge that can be

reverse-evaluated from the following computationally-determined plot:

Figure 9: A plot of polarization energy times nanocrystal radius against = CdSeoutside

, where

outside is the permittivity of the solvent around the nanocrystal (in this case, octadecene,for which outside = 1.9

[3]).

Using CdSe = 10.6 and outside = 1.9 and looking at Figure 9, we can determine that

Epol(eV) 0.8R(A) . Plugging everything into the two equations and summing the two terms,

we can calculate the minimum excitation energies per particle:

7

Sample Radius (nm) Epol (eV) Eex Epol (eV) Eex (eV)Sample 1 1.12(1) 0.071(2) 2.8(3) 2.9(4)Sample 2 1.19(1) 0.067(3) 2.4(2) 2.5(1)Sample 3 1.25(1) 0.064(2) 2.2(1) 2.3(1)Sample 4 1.33(1) 0.060(1) 1.9(1) 2.0(1)Sample 5 1.38(2) 0.058(1) 1.8(1) 1.8(1)Sample 6 1.40(2) 0.057(1) 1.7(1) 1.8(1)

Table 4: Nanocrystal excitation energies, calculated from their radii and an extension ofthe particle-in-a-box equation.

The uncertainty propagation equation for this equation is

Eex =

((h2

8

(1

me+

1

mh

))(RR

)(2R)

)2+

((1.8e2

4CdSe0

)(RR

)(R)

)2,

taking into account only errors in the radius and assuming all fundamental constants,

literature values, and computational estimates have no intrinsic error.

References

[1] Yu, W. W., Qu, L., Guo, W., Peng, X. Chem. Mater. 15:2854 (2000)

[2] Kippeny, T., Swafford, L. A., Rosenthal, S. J.J. Chem. Ed. 79:1094 (2002)

[3] List of common solvents by dielectric constant and refractive index.

http://www.stenutz.eu/chem/solv23.php

[4] Shoemaker, Garland, Nibler. Experiments in Physical Chemistry, 8th ed.; 2008.

8

Recommended